IEEE TRANSACTIONS ON MAGNETICS, VOL. 41, NO. 2, FEBRUARY 2005 903 Study of Magnetic Properties and Local Structures in Discontinuous-CoFe–ZnO Multilayers H. S. Hsu, J. C. A. Huang, Lance Horng, C. H. Lee, Y. H. Huang, Y. F. Liao, and M. Z. Lin A Abstract—In this study, we have investigated the magnetic properties and local structures of discontinuous-Co70 Fe30 (x )–ZnO multilayers (MLs). With the variation of Co70 Fe30 nominal thickness, the phase transition from diluted magnetic semicon, ML, to granular phase, ductor (DMS) phase, and 9 MLs, is indicated from the measurements of magnetization versus temperature behavior and extended X-ray absorption fine structure (EXAFS) on Co or Fe K-edge. The analysis of EXAFS at Zn K-edge shows the reduction of Co coordination numbers with the increasing CoFe thickness. This result demonstrates that the CoFe grain size plays an important role in the formation of DMS and is greatly critical for multilayer growth technique. =1 =5 Index Terms—Diluted magnetic semiconductor (DMS), discontinuous multiplayer, extended X-ray absorption fine structure (EXAFS). I. INTRODUCTION D ILUTED MAGNETIC semiconductors (DMSs) have been of much interest and studied extensively since Dietl et al.  predicted room temperature (RT) ferromagnetism can be induced by doping transition metal (TM) elements into host semiconductors. Especially, TM-doped ZnO has been investigated as a promising DMS for implementing spintronics and optoelectronics device . In spite of TM atomic substitution for Zn ions, the origin of RT ferromagnetism remains controversial. Most of the studies emphasized the magnetic elements concentration in the host semiconductor , but the grain size effect of doping magnetic element in fabrication process has not been particularly discussed. In this paper, we investigate the magnetic properties and local structures of Co Fe –ZnO multilayers (MLs). Here, the inserted CoFe layers are discontinuous because the thickness nm) is below the minimum value of a continuous film. By ( varying the deposition thickness, the grain size distribution of Co Fe can be controlled , where CoFe was chosen to study the difference of reaction in ZnO matrix between Co and Fe atom. The magnetic origin relating to the local structures Manuscript received August 21, 2004. This work was supported in part by the Taiwan National Science Foundation under Grant NSC 92-2120-M-006-006. H. S. Hsu is with the Department of Physics, National Cheng Kung University, Tainan 701, Taiwan, R.O.C. (e-mail: [email protected]). J. C. A. Huang is with the Department of Physics, National Cheng Kung University, Tainan 701, Taiwan, R.O.C. and also with the Department of Applied Physics, National University of Kaohsiung, Kaohsiung 003, Taiwan, R.O.C. (e-mail: [email protected]). L. Horng is with the Department of Physics, National Changhua University of Education, Changhua 500, Taiwan, R.O.C. (e-mail: [email protected]). C. H. Lee, Y. H. Huang, Y. F. Liao, and M. Z. Lin are with the Department of Engineering and System Science, National Tsing Hua University, Hsinchu 300, Taiwan, R.O.C. (e-mail: [email protected]). Digital Object Identifier 10.1109/TMAG.2004.842085 surrounding Co and Fe are discussed. The size effect of the magnetic elements is also studied by extended X-ray absorption fine structure (EXAFS) spectra at Zn K-edge. We present our study on the variation of CoFe grain size to understand the related mechanism of DMS. II. EXPERIMENT We have prepared [discontinuous-Co Fe (x )–ZnO (20 )] multilayers by ion-beam sputtering with a base pressure of 8 10 torr. The nominal thickness of Co Fe layers were and . Sputtering was executed in an atmosphere of 2 10 torr with Ar ion beam acting alternatively on CoFe and ZnO targets. All films were deposited on Al O (0001) single crystal substrates for good epitaxial structure. The deposition rate was calibrated to achieve uniform values of 0.2 /s for ZnO and 0.5 /s for CoFe. Measurements of the as a function of magnetic field and magnetization were characterized with a superconducting temperature quantum interference device (SQUID) magnetometer over a temperature range of 6 K–350 K. In order to investigate the electronic states and local structure of ZnO–CoFe MLs, X-ray absorption spectroscopy on Co, Fe, and Zn K-edges was carried out at the wigger beamline of the Synchrotron Radiation Research Center, Hsinchu, Taiwan. III. RESULTS AND DISCUSSION Fig. 1 shows the magnetization versus applied field (M–H) curves of the three MLs measured at 300 K. Magnetic hysteresis and MLs. In contrast, paraloops were observed for ML. Note that the magnetic linear relation appears for ML is much larger than ML. It imcoercivity of plies the origin of RT ferromagnetism between and MLs may be different, as discussed in the following. Fig. 2 displays the zero-field-cooling (ZFC) and field-cooling (FC) magnetization measurements as a function of temperature , and MLs. (M–T) in a low field of 50 Oe for the ML, the FC magnetization remains almost constant For and does not decrease to zero up to 350 K. Besides, the peak which is a signature for blocking temperature does not appear ML. This suggests that the CoFe in the ZFC curve for atoms are dissolved into ZnO matrix and forms DMS without any formation of magnetic clusters. ML, both and MLs show In contrast to magnetic blocking phenomenon in their ZFC curves. It clearly evidences the presence of magnetic clusters in ZnO matrix for and MLs. Note that moves to higher tem( K) to perature as CoFe layer increased from 0018-9464/$20.00 © 2005 IEEE 904 IEEE TRANSACTIONS ON MAGNETICS, VOL. 41, NO. 2, FEBRUARY 2005 Fig. 3. Fourier transform of EXAFS for x and ZnO at Zn K-edge, respectively. A)–Co Fe (x A)] as Fig. 1. Magnetization of the multilayers [ZnO(20 a function of applied magnetic field at 300 K for (a) x = 1, (b) x = 5, and (c) x = 9 MLs. The inset is the zoom in figure of (c). Fig. 2. ZFC (solid symbol)-FC (hollow symbol) M–T curve in a field of 50 Oe for (a) x = 1, (b) x = 5, and (c) x = 9 MLs. ( K), suggesting that the average size of clusters increases with the CoFe nominal thickness. The FC curve ML displays the typical Curie–Weiss behavior for for disordered granular systems and the magnetization approaches to zero at RT. The linear relation of M–H loop in Fig. 1(b) is characteristic of the predominant paramagnetic phase contributed by blocked magnetic nanoparticles. The M–T behavior = 1 5 9 MLs at Co, Fe K-edge, ; ; of ML is similar to ML even if the M–H behavML iors at RT are different. The RT ferromagnetism for should be caused by the magnetic clusters, in contrast to the inML. trinsic DMS property for Fig. 3 compares the radial distribution function (RDF), the Fourier transforms amplitude from EXAFS data on Co, Fe, and Zn K-edges for MLs and pure ZnO. For ML, the interatomic distances for the two major peaks of the film are essentially the same as undoped ZnO both on Co and Fe K-edge. The first and second major peaks are corresponding to the nearest oxygen and Zn (or Co, Fe) atoms from a specific Co ML reveals that most (Fe) atom. Accordingly, the RDF of Co (Fe) atoms substitute for Zn atoms without precipitating magnetic clusters. It further supports that the origin of RT ferroML is due to an intrinsic DMS effect. For magnetism for ML, essentially only one major peak has been observed at Co K-edge, indicating in average Co atoms locate at 2 from nearest Co atoms, or the formation of Co metal clusters. On ML reveals the other hand, the RDF of Fe K-edge for only a nearest-neighbor (oxygen) shell and does not have any long-range structural order surrounding with Fe atoms. These results reveal the Co and Fe atoms play different contribution when precipitate in ZnO matrix. Similar EXAFS results were ML. Therefore, the magnetic blocking beobtained for and MLs could be mainly caused by Co clushavior for ters, not by Fe cluster. Using the literature values of versus size , we estimate the average size of the Co nanoparticles in ML and about 8 nm for our samples are about 1 nm for ML. The RT ferromagnetism for ML could originate from the large unblocked Co nanoparticles. , and MLs Fig. 4 shows the Fourier transforms of from the Zn K-edge EXAFS data. The two pronounced peaks for all samples are located at the resemble values. It is noted that are slightly the magnitudes of the second shell peaks 3.0 reduced with increasing the CoFe thickness. It means that the second nearest neighbor surrounding with Zn atoms (Zn, Co, , and MLs. The quantitative or Fe) is different for local structure information was obtained by curve fitting (solid curves) from theoretical models generated by the well-known HSU et al.: STUDY OF MAGNETIC PROPERTIES AND LOCAL STRUCTURES IN DISCONTINUOUS-CoFe–ZnO MULTILAYERS 905 nation numbers are less than 1 for all MLs, particularly clear ML. The origin of low Fe solubility is not clear so for far. Fe may be stable in the trivalent state in ZnO, resulting in ML shows of the low solubility limit . Besides, and MLs have only 0.52 and 2.83 Co atoms, while 0.64 Co atoms, respectively. The reduction of Co coordination numbers results in a less incorporation in ZnO matrix without ever reaching to saturation condition. This indicates that the increase of CoFe nominal thickness ( ) does not increase in magnetic doping concentration if the magnetic elements exceed a . These results suggest that the struccritical thickness ture and magnetism of discontinuous-CoFe/ZnO multilayers is very sensitive to nominal CoFe thickness because of the variation in solubility. The control of inserting magnetic grain size distribution can stabilize or destroy the DMS phase. IV. CONCLUSION Fig. 4. Fourier transforms of EXAFS at Zn K-edge (hollow symbols) and fitting results (solid curves) from FEFF code for (a) x = 1, (b) x = 5, and (c) x = 9 MLs. TABLE I RESULTS OF FITS TO x = 1; 5, AND 9 MLs. Zn-O PAIR IS THE FIRST COORDINATION SHELL AND Zn-Zn PAIR IS THE SECOND COORDINATION SHELL. N IS THE COORDINATION NUMBER, R IS THE DISTANCE BETWEEN CENTERED Zn ATOMS AND COORDINATION ATOMS, AND IS THE MEAN SQUARE DISORDER AT ROOM TEMPERATURE We have performed systematical study of magnetic properties and local structures of Co, Fe, and Zn in discontinuousCoFe/ZnO multilayers. By varying in Co Fe nominal thickness, the two-step magnetic phase transition from RT ferromag, paramagnetism and to RT ferromagnetism netism have been observed. The measurements on M–T behavior and EXAFS on Co (Fe) edge further indicate that the ML originates from observed RT ferromagnetism for an intrinsic DMS phase, whereas the RT ferromagnetism for ML is caused by large unblocked Co nanoparticles. This result could be associated with varying dimensionality between magnetic clusters, evidenced by the quantitative local structure information at Zn K-edge. REFERENCES FEFF program. The solid curves in Fig. 4 are obtained by the best fit of the experimental data, which reveal reasonably good agreement of the theoretical model with the data. For convenience, the fitting results are summarized in Table I. For the first coordination shell, all three samples have the 4 within the error bar for the same coordination number Zn-O pair. For the second coordination shell, the Fe coordi-  K. Sato and H. Katayama-Yoshida, “Stabilization of ferromagnetic states by electron doping in Fe-, Co-or Ni-doped ZnO,” Jpn. J. Appl. Phys., pt. 2, vol. 40, pp. L334–L336, 2001.  S. A. Wolf, D. D. Awschalom, R. A. Buhrman, J. M. Daughton, S. von Molnar, M. L. Roukes, A. Y. Chthekanova, and D. M. Treger, “Spintronics: A spin-based electronics vision for the future,” Science, vol. 294, pp. 1488–1495, 2001.  J. H. Park, M. G. Kim, H. M. Jang, S. Ryu, and Y. M. Kim, “Co-metal clustering as the origin of ferromagnetism in co-doped ZnO thin films,” Appl. Phys. Lett., vol. 84, pp. 1338–1340, 2004.  G. N. Kakazei, Y. G. Pogorelov, A. M. L. Lopes, J. B. Sousa, S. Cardoso, P. P. Freitas, M. M. Prerira de Azevedo, and E. Snoeck, “Tunnel magnetoresistance and magnetic ordering in ion-beam sputtered Co Fe –Al O discontinuous multilayers,” J. Appl. Phys, vol. 90, pp. 4044–4048, 2001.  J. P. Chen, C. M. Sorensen, K. J. Klabunde, and G. C. Hadjipanayis, “Enhanced magnetization of nanoscale colloidal cobalt particles,” Phys. Rev. B, Condens. Matter, vol. 51, pp. 11 527–11 532, 1995.  R. Heitz, A. Hoffmann, and I. Broser, “Fe center in ZnO,” Phys. Rev. B, Condens. Matter, vol. 45, pp. 8977–8988, 1992.